PEABODY’SCONTROL OF PIPELINE CORROSIONSECOND EDITIONA.W. PEABODYEdited byRONALD L. BIANCHETTI NACE International The Corrosion Society 1440 South Creek Drive Houston, Texas 77084
NACE International The Corrosion Society C 1967, 2001 by NACE International Second Edition 2001. All rights reserved. Library of Congress Catalog Number 99-80032 ISBN 1-57590-092-0Printed in the United States of America. All rights reserved. This book, or parts thereof,may not be reproduced in any form without permission of the copyright owners.Neither NACE International, its ofﬁcers, directors, or members thereof accept any re-sponsibility for the use of the methods and materials discussed herein. The informationis advisory only and the use of the materials and methods is solely at the risk of the user. Cover illustration by Mark Lewis, courtesy of the East Bay Municipal Utility District. NACE Press: Director of Publications: Jeff Littleton Manager of NACE Press: Neil Vaughan NACE International 1440 South Creek Drive Houston, Texas 77084 http://www.nace.org
Table of Contents Preface v About the Author vii Contributors ixChapter 1 Introduction to Corrosion John A. Beavers 1Chapter 2 Pipeline Coatings Richard N. Sloan 7Chapter 3 Cathodic Protection—How It Works John A. Beavers 21Chapter 4 Criteria for Cathodic Protection John A. Beavers and Kevin C. Garrity 49Chapter 5 Survey Methods and Evaluation Techniques Ronald L. Bianchetti 65Chapter 6 Instrumentation Mark Lewis 101Chapter 7 Ground Bed Design Ronald L. Bianchetti 131Chapter 8 Impressed Current Cathodic Protection Ronald L. Bianchetti 157 iii
iv Table of ContentsChapter 9 Cathodic Protection with Galvanic Anodes Ronald L. Bianchetti 177Chapter 10 Cathodic Protection with Other Power Sources John A. Beavers 201Chapter 11 Stray Current Corrosion Michael J. Szeliga 211Chapter 12 Construction Practices Ronald L. Bianchetti 237Chapter 13 Maintenance Procedures Ronald L. Bianchetti 261Chapter 14 Microbiologically Inﬂuenced Corrosion Brenda J. Little and Patricia Wagner 273Chapter 15 Economics Ronald L. Bianchetti 285Chapter 16 Fundamentals of Corrosion John A. Beavers 297Appendix A NACE Glossary of Corrosion-Related Terms 319Appendix B Additional Important Information on Underground Corrosion Control 339 Index 341
Preface This book was originally published in 1967 by Sam Peabody and is the most quoted and used document in the corrosion industry for pipeline corrosion control and testing. When the original book was published, speciﬁc criteria for cathodic protection for underground pipelines were still under evaluation and consideration. Not until 1969 was the ﬁrst documented standard approved by NACE International on criteria RP0169. The depth and vision that Peabody incorporated in the ﬁrst version of the book has stood the test of time. This revised version of the 1967 book is not an attempt to make radical changes to the original document. Much of the original text and concepts remain intact. We attempted, however, to incorporate original traditional elements of the book with updates and expanded discussions on equipment, testing techniques and criteria, coatings, survey methods, and data analysis. An integral part of this revision is a CD-ROM that contains formulas of key design calculations, case examples of corrosion control designs which provide a set-by-step overview of how to design various components of cathodic protection systems, and an electronic copy of the revised book edition. As described in the Preface of the original 1967 edition, every attempt has been made to check the accuracy of all statements and other data. However, it is unreasonable to assume that everything in this book is accurate and exact. Any suggestions will be considered when future editions of this book are prepared. v
About the Author 1915–1998 This updated version of NACE International’s book titled Control of Pipeline Corrosion is dedicated to the memory of its original author, A.W. (Sam) Peabody. Since its publication in 1967, the book has been translated into at least seven different languages and is considered by most as the deﬁnitive work on pipeline corrosion. Sam received his bachelor’s degree from the University of Maine and pursued grad- uate studies at the Brooklyn Polytechnic Institute in New York. He worked for Ebasco Services Inc. (no longer in existence) for over 40 years until his retirement in 1980 as Director of Corrosion Engineering. He was an active member of NACE since 1947. His accomplishments, awards, and recognitions are too many to list here. His biggest legacy, especially to those of us who had the privilege of working for and with him, is that he was the perfect example of “a gentleman and a scholar.” He was an excellent teacher who always emphasized professional integrity, a quality he instilled in so many. vii
ContributorsJohn A. Beavers John A. Beavers is Vice President of Research at CC Technologies, a corrosion engineering and research company. He received B.S. and Ph.D. degrees in metallurgical engineering from the University of Illinois at Urbana-Champaign in 1973 and 1977, respectively. Dr. Beavers has directed and contributed to numerous research programs on corrosion performance of structural materials. These programs included failure analyses, critical literature reviews, and laboratory and ﬁeld evaluations of metallic and non-metallic material. Dr. Beavers has utilized state-of-the-art electrochemical, surface analytical, and mechanical techniques for the evalua- tion of materials performance. A major emphasis of his research has been the mechanistic and practical aspects of corrosion and stress corrosion cracking (SCC) on underground pipelines. Dr. Beavers worked at Battelle Memorial Institute from 1977 to 1987, where he was a Senior Research Leader in the Corrosion Section. He joined CC Technologies in 1987. Dr. Beavers has authored over 80 papers in the ﬁeld of corrosion and has received two U.S. Patents. An active member of NACE, he was Chairman of the Research in Progress Symposium in 1994 and of the Publications Committee in 1991 and 1992. Editor’s Note: Sincere appreciation to John Beavers for investing a lot of time on a detailed and productive review of the ﬁnal draft on the eve before printing.Ronald L. Bianchetti Ronald L. Bianchetti is currently a Senior Engineer at East Bay Municipal Utility District (EBMUD) in Oakland, California. He received a B.S. in engineering in 1975 from the University of California, Davis and an MBA in 1981 from St. Mary’s College of California. He is a Registered Professional Engineer and has over 25 years of experience. Prior to holding his current position, Mr. Bianchetti worked in the private sector as a consultant in the cor- rosion industry from 1975 to 1992. His work includes planning, designing, testing, and the construction management of cathodic protection systems for underground pipelines, tanks, reﬁneries, power plants, and marine structures. He has served in NACE International as Past ix
x Contributors Chairman of the Publications Committee, ad-hoc member to the Board of Directors, Past Western Region Chairman and Past Section Chair of the San Francisco Section. Mr. Bianchetti has published over 30 papers in the ﬁeld of corrosion and has given hun- dreds of presentations on corrosion and corrosion control.Kevin C. Garrity, P.E. Kevin C. Garrity, P.E., is currently Vice President of Engineering at CC Technologies, a cor- rosion engineering and research company. He received a B.S. in electrical engineering in 1974 from the Polytechnic Institute of Brooklyn. He is a NACE Certiﬁed Cathodic Protection Specialist and a Registered Professional Engineer in seven states. Mr. Garrity has 26 years of experience in the design, installation, monitoring, and assessment of cathodic protection systems for buried pipelines, underground storage tanks, concrete structures, and marine structures. Mr. Garrity worked at Ebasco Services from 1974 to 1982, where he was a Senior Corrosion Engineer, and at Harco Corporation from 1982 to 1989, where he was Vice President of Engineering. He joined CC Technologies in 1989. In 1996, Mr. Garrity received the Colonel George W. Cox Award for outstanding contribu- tions to the ﬁeld of underground corrosion control. He has published more than 20 papers in the ﬁeld of corrosion control. Mr. Garrity delivered the plenary lecture at Corrosion’98.Mark Lewis Mark Lewis is Assistant Corrosion Engineer at the East Bay Municipal Utility District (EBMUD) in Oakland, California. He is a graduate of Kent State University and attended Bethany College in West Virginia. He has worked in the cathodic protection and corrosion engineering ﬁeld since 1980, both within the United States and internationally. He is a Past Chairman of the San Francisco Bay Area Section of NACE International. He is the author of several technical and historical articles on cathodic protection and has made numerous presentations on the subject. Mr. Lewis has a patent pending for a distribution system rectiﬁer design.Brenda J. Little Brenda J. Little, Senior Scientist for Marine Molecular Processes at the Naval Research Labora- tory, has a Ph.D. in chemistry from Tulane University and a B.S. in biology and chemistry from Baylor University. She is a member of the American Chemical Society and the National As- sociation of Corrosion Engineers (NACE International). She is a NACE International Fellow and the recipient of a 1999 NACE International Technical Achievement Award. Dr. Little serves on the editorial board for Biofouling and is the author of one book, 20 book chapters, and over 80 peer-reviewed journal articles.
Contributors xiSteve McKim Since 1989, Steve McKim has been Vice President of American Construction & Supply, Inc. Based in Mill Valley, California, his company specializes in cathodic protection construction services. Mr. McKim previously worked with Harco Corporation and Chevron USA. He has been in the corrosion industry since he graduated from the University of Illinois with a B.S. in mechanical engineering in 1983. He is a Past Chairman of the NACE San Francisco Bay Area Section.Richard N. Sloan The late Richard Sloan, was an authority in the ﬁeld of pipeline coatings. He worked for over 45 years with a company that was ﬁrst known as HC Price. (The company changed its name several times: HC Price, Ameron Price, Bredero Price, and Energy Coatings.) He attended Drexel University and graduated with a bachelor’s degree in Industrial Administration. During his professional career, Richard Sloan taught various short courses in pipeline coatings, and was a speaker at numerous seminars on the subject. The late Mr. Sloan was an active and long-standing member of NACE, AWWA, and Western Pipeliners.Michael J. Szeliga Michael J. Szeliga, P.E., is the Chief Engineer for Russell Corrosion Consultants, Inc. He has more than 23 years of experience in corrosion control engineering. Much of his work has involved the analysis and control of stray current from DC-powered transit systems and from impressed current cathodic protection systems. A Licensed Professional Engineer in several states and certiﬁed by NACE International as a Corrosion Specialist and a Cathodic Protection Specialist, Mr. Szeliga has been and is the principal corrosion consultant for the design, construction, and maintenance of many light and heavy rail transit systems. He is presently chairman of the NACE (05)024X Committee on Interference Problems Associated with Rail Transit. Mr. Szeliga is also chairman of the ASTM subcommittee on stray current. He has edited a book for NACE International titled Stray Current Corrosion and has pub- lished several articles on the subject.Patricia Wagner Patricia Wagner retired from the Naval Research Laboratory in 1998 after 14 years of extensive experience in microbiologically inﬂuenced corrosion. She is the coauthor of one book and the author of numerous articles on corrosion.
1 Chapter Introduction to Corrosion John A. BeaversWHAT IS CORROSION? One general deﬁnition of corrosion is the degradation of a material through environ- mental interaction. This deﬁnition encompasses all materials, both naturally occurring and man-made and includes plastics, ceramics, and metals. This book focuses on the corrosion of metals, with emphasis on corrosion of carbon and low-alloy steels used in underground pipelines. This deﬁnition of corrosion begs the question; why do met- als corrode? The answer lies in the ﬁeld of thermodynamics, which tells whether a process such as corrosion will occur. A second logical question is what is the rate of corrosion or how long will a pipeline last? Corrosion kinetics can help provide an answer to this question. Both topics are discussed in greater detail in Chapter 16. Chap- ter 1 contains an introduction to the subject of underground corrosion. A glossary of terms is included in Appendix A of this book to help with the sometimes confusing terminology. A signiﬁcant amount of energy is put into a metal when it is extracted from its ores, placing it in a high-energy state. These ores are typically oxides of the metal such as hematite (Fe2 O3 ) for steel or bauxite (Al2 O3 ·H2 O) for aluminum. One principle of thermodynamics is that a material always seeks the lowest energy state. In other words, most metals are thermodynamically unstable and will tend to seek a lower energy state, which is an oxide or some other compound. The process by which metals convert to the lower-energy oxides is called corrosion. Corrosion of most common engineering materials at near-ambient temperatures oc- curs in aqueous (water-containing) environments and is electrochemical in nature. The aqueous environment is also referred to as the electrolyte and, in the case of under- ground corrosion, is moist soil. The corrosion process involves the removal of elec- trons (oxidation) of the metal [Equation (1)] and the consumption of those electrons by some other reduction reaction, such as oxygen or water reduction [Equations (2) and (3), 1
2 Introduction to Corrosion respectively]: Fe → Fe++ + 2e− (1) − − O2 + 2H2 O + 4e → 4OH (2) 2H2 O + 2e− → H2 + 2OH− (3) The oxidation reaction is commonly called the anodic reaction and the reduction reaction is called the cathodic reaction. Both electrochemical reactions are necessary for corrosion to occur. The oxidation reaction causes the actual metal loss but the reduction reaction must be present to consume the electrons liberated by the oxidation reaction, maintaining charge neutrality. Otherwise, a large negative charge would rapidly develop between the metal and the electrolyte and the corrosion process would cease. The oxidation and reduction reactions are sometimes referred to as half-cell reactions and can occur locally (at the same site on the metal) or can be physically separated. When the electrochemical reactions are physically separated, the process is referred to as a differential corrosion cell. A schematic of a differential corrosion cell is given in Figure 1.1. The site where the metal is being oxidized is referred to as the anode or anodic site. At this site, direct electric current (deﬁned as a positive ﬂow of charge) ﬂows from the metal surface into the electrolyte as the metal ions leave the surface. This current ﬂows in the electrolyte to the site where oxygen, water, or some other species is being reduced. This site is referred to as the cathode or cathodic site. There are four necessary components of a differential corrosion cell. 1. There must be an anode 2. There must be a cathode Figure 1.1 Schematic showing a differential corrosion cell.
How Do We Detect Corrosion? 3 3. There must be a metallic path electrically connecting the anode and cathode. (Nor- mally, this will be the pipeline itself.) 4. The anode and cathode must be immersed in an electrically conductive electrolyte (normally, moist soil). Underground corrosion of pipelines and other structures is often the result of differ- ential corrosion cells of which a variety of different types exist. These include differential aeration cells, where different parts of a pipe are exposed to different oxygen concen- trations in the soil, and cells created by differences in the nature of the pipe surface or the soil chemistry. Galvanic corrosion is a form of differential cell corrosion in which two different metals are electrically coupled and exposed in a corrosive environment. Further discussion of these differential corrosion cells is given below and in Chapter 16.HOW DO WE DETECT CORROSION? The electrochemical nature of the corrosion process provides opportunities to detect and mitigate corrosion of underground structures. We can monitor the voltages and the currents associated with the corrosion process. When a piece of metal is placed in an electrolyte, such as soil, a voltage will develop across the metal–electrolyte interface because of the electrochemical nature of the cor- rosion process. We cannot measure this voltage directly but, using a voltmeter, we can measure a voltage between two different metals that are placed in the soil. We also can measure the voltage difference between a metal and a reference electrode, commonly called a half-cell electrode. This voltage is referred to as a corrosion potential, an open circuit potential, or a native potential for that metal in the environment in which the mea- surement is being obtained. For soil environments, the most common reference electrode used is the copper–copper sulfate reference electrode (CSE). Potential measurements can be used to estimate the relative resistance of different metals to corrosion in a given environment. Noble metals, such as gold and platinum, have more positive potentials and are more resistant to corrosion than are the more common engineering metals such as steel and aluminum. A galvanic series is a list of metals and alloys arranged according to their relative corrosion potentials in a given environment. Table 1.1 shows a galvanic series for metals and other materials in neutral soils and water, indicating that carbon has the most positive potential of the materials listed and magnesium has the most negative potential. The potentials measured for the different metals in a galvanic series vary somewhat, depending on the nature of the environment, but the relative position of the metals is similar for natural environments such as soil and seawater. Another use for corrosion potential measurements is to establish whether galvanic corrosion is likely to occur. When two metals are electrically coupled in an environ- ment, the more negative (active) member of the couple will become the anode in the
4 Introduction to Corrosion Table 1.1 Practical Galvanic Series for Materials in Neutral Soils and Water Material Potential Volts (CSE)a Carbon, Graphite, Coke +0.3 Platinum 0 to −0.1 Mill Scale on Steel −0.2 High Silicon Cast Iron −0.2 Copper, Brass, Bronze −0.2 Mild Steel in Concrete −0.2 Lead −0.5 Cast Iron (Not Graphitized) −0.5 Mild Steel (Rusted) −0.2 to −0.5 Mild Steel (Clean and Shiny) −0.5 to −0.8 Commercially Pure Aluminum −0.8 Aluminum Alloy (5% Zinc) −1.05 Zinc −1.1 Magnesium Alloy (6% Al, 3% Zn, 0.15% Mn) −1.6 Commercially Pure Magnesium −1.75 a Typical potential normally observed in neutral soils and water, mea- sured with respect to copper sulfate reference electrode. differential corrosion cell, and the more positive (noble) member of the couple will be- come the cathode in the cell. In general, the severity of the galvanic couple increases as the difference in potential between the two members of the couple increases, although this is not always the case. The galvanic series shown in Table 1.1 indicates that, where copper is electrically coupled to mild steel in soil, the copper will become the cathode and the steel will become the anode, accelerating corrosion of the steel. A further discussion of galvanic corrosion is given in Chapter 16. Table 1.1 also shows that the potential of mild steel can differ depending on whether the surface is clean or covered with mill scale. The potential of steel also is a function of soil properties, including pH, ion concentration, oxygen, and moisture content. The po- tential differences that develop on underground pipelines and other structures as a result of these factors can result in severe corrosion. Further discussions of these differential corrosion cells are given in Chapter 16. Potential measurements are commonly used on underground pipelines to detect the presence of these types of differential corrosion cells. An electrical connection is made to the pipe, and the potential of the pipe is measured with respect to a reference electrode placed over the pipe. This process is shown schematically in Figure 1.2. Normally, the reference electrode is connected to the negative lead of a digital voltmeter to obtain a negative reading. As shown in Table 1.1, most potentials in soils are negative. With this type of measurement, the most negative regions of the structure are the anodes and are undergoing accelerated corrosion due to the differential corrosion cells.
How Do We Mitigate Corrosion? 5 Figure 1.2 Schematic showing a pipe- to-soil potential measurement. Current measurements also can be used to detect differential corrosion cells if the anodes and cathodes are large. These large cells create long-line currents that can be detected by measurements made over the pipe or other underground structure. Through Ohm’s law (V = IR, where V is the voltage, I is the current, and R is the resistance) we know that current ﬂow in the soil will create a voltage gradient. This gradient can be detected by placing identical reference electrodes over the pipe and measuring the voltage difference. The voltage measurements can be used to indicate the direction of the differential cell current. The anodic and cathodic sites on the pipeline can be located by performing a series of cell-to-cell potential measurements taken along the pipeline. Another possible source of current ﬂow in the ground is stray currents. These issues are discussed further in Chapter 5.HOW DO WE MITIGATE CORROSION? The principal methods for mitigating corrosion on underground pipelines are coatings and cathodic protection (CP). Although each will be treated in greater detail in the following chapters, these two methods are brieﬂy described here.
6 Introduction to Corrosion Coatings normally are intended to form a continuous ﬁlm of an electrically insulating material over the metallic surface to be protected. The function of such a coating is to isolate the metal from direct contact with the surrounding electrolyte (preventing the electrolyte from contacting the metal) and to interpose such a high electrical resistance that the electrochemical reactions cannot readily occur. In reality, all coatings, regardless of overall quality, contain holes, referred to as holidays, that are formed during appli- cation, or during transport or installation of mill-coated pipe. Holidays in coatings also develop in service as a result of degradation of the coating, soil stresses, or movement of the pipe in the ground. Degradation of the coating in service also can lead to disbonding from the pipe surface, further exposing metal to the underground environment. A high corrosion rate at a holiday or within a disbonded region can result in a leak or rupture, even where the coating effectively protects a high percentage of the pipe surface. Thus, coatings are rarely used on underground pipelines in the absence of CP. The primary function of a coating on a cathodically protected pipe is to reduce the surface area of exposed metal on the pipeline, thereby reducing the current necessary to cathodically protect the metal. Further discussion of coatings is given in Chapter 2. One deﬁnition of CP is a technique to reduce the corrosion rate of a metal surface by making it the cathode of an electrochemical cell. This is accomplished by shifting the potential of the metal in the negative direction by the use of an external power source (referred to as impressed current CP) or by utilizing a sacriﬁcial anode. In the case of an impressed current system, a current is impressed on the structure by means of a power supply, referred to as a rectiﬁer, and an anode buried in the ground. In the case of a sacriﬁcial anode system, the galvanic relationship between a sacriﬁcial anode material, such as zinc or magnesium, and the pipe steel is used to supply the required CP current. Further discussions of CP are given in Chapters 3 and 16.
2 Chapter Pipeline Coatings Richard N. Sloan When the ﬁrst edition of Control of Pipeline Corrosion by A.W. Peabody was published in 1967, there were few governmental regulations to contend with. Today the Department of Transportation–Ofﬁce of Pipeline Safety (DOT/OPS), Occupational Safety and Health Administration (OSHA), and the Department of Environmental Resources (DER) are among the many regulatory agencies inﬂuencing or controlling the pipeline industry. Governmental regulations, along with the development, introduction, and acceptance of new pipeline coatings, have made major changes and will continue to affect the selection and use of pipeline coatings in the future. Economics, while still a factor, is being replaced by safety and environmental con- cerns to obtain the best available pipe-coating systems. This trend was ﬁrst apparent in Europe where permanence, instead of cost, led to the use of multi-layer systems that have proven to be most effective and more economical over the life of the pipeline. In today’s regulated environment, all new hazardous pipelines (carrying oil, gas, or other potentially dangerous substances) are required by federal regulation to use an effective coating and cathodic protection (CP).EFFECTIVENESS OF COATINGS AS A MEANS OF CORROSION CONTROL First attempts to control pipeline corrosion relied on the use of coating materials and the reasoning that if the pipeline metal could be isolated from contact with the surrounding earth, no corrosion could occur. This concept is entirely reasonable and logical. Further- more, a coating would be completely effective as a means of stopping corrosion if the coating material: • Is an effective electrical insulator, 7
8 Pipeline Coatings • Can be applied with no breaks whatsoever and will remain so during the backﬁlling process, and • Constitutes an initially perfect ﬁlm that will remain so with time. While this is possible with some of the advanced multi-layer systems, it may not be practical from an initial cost analysis. Although coatings by themselves may not be the one perfect answer to corrosion control, they are extremely effective when properly used. Most operators plan coatings and cathodic protection (CP) for all their pipelines as a matter of course. A properly selected and applied coating will provide all the protection necessary on most of the pipeline surface to which it is applied. On a typical well-coated pipeline this should be better than 99% and, along with the CP, should give total protection. It is not the intent of the chapter to make speciﬁc recommendations for coating ma- terials to be used. However, the capabilities and limitations of various pipeline coating materials will be discussed as well as desirable characteristics and how to get the most of any material used. Types of coatings now used on pipeline systems will be described brieﬂy. NACE Standard RP0169-96 Section 5: Coatings, is a comprehensive guide to pipe coatings, and is required reading for a better understanding of their importance. This Standard lists the following desirable characteristics of coatings: 1. Effective electrical insulator. Because soil corrosion is an electrochemical process, a pipe coating has to stop the current ﬂow by isolating the pipe from its installed environment/electrolyte. To assure a high electrical resistance, the coating should have a high dielectric strength. 2. Effective moisture barrier. Contrary to the theory that water absorption is good because it increases the effectiveness of CP, water transfer through the coating may cause blistering and will contribute to corrosion by prohibiting isolation. 3. Applicability. Application of the coating to the pipe must be possible by a method that will not adversely affect the properties of the pipe and with a minimum of defects. 4. Ability to resist development of holidays with time. After the coating is buried, two areas that may destroy or degrade coatings are soil stress and soil contaminants. Soil stress, brought about in certain soils that are alternately wet and dry, creates forces that may split or cause thin areas. To minimize this problem, one must evaluate the coating’s abrasion resistance, tensile strength, adhesion, and cohesion. The coating’s resistance to chemicals, hydrocarbons, and acidic or alkaline conditions should be known for evaluating their performance in contaminated soils. 5. Good adhesion to pipe surface. The pipe coating requires sufﬁcient adhesion to prevent water ingress or migration between the coating and the pipe, along with cohesion to resist handling and soil stress. Soil stress is the main cause of pipe coat- ing failure. “Soil stress effects can be seen on ﬂexible PE coatings with elastomeric adhesives as a characteristic wrinkling. However, other types of coatings can fail by blistering fusion-bonded epoxy (FBE) or fatigue cracking coal tar enamel (CTE)
Effectiveness of Coatings as a Means of Corrosion Control 9 that are exacerbated by soil movement. . . . resistance to shear must be combined with a measurement of the resistance of the backing material (or outer jacket) to deformation and tensile force. The two properties combine to determine the ability of a pipeline coating to resist damage to soil movement.” Soil stress resistance is measured by shear resistance, not by peel strength. 6. Ability to withstand normal handling, storage (UV degradation), and installation. The ability of a coating to withstand damage is a function of its impact, abrasion, and ﬂexibility properties. Pipe coatings are subject to numerous handlings between application and backﬁll. Their ability to resist these forces vary considerably, so those factors need to be evaluated to know if any special precautionary measure should be used. Ultraviolet rays can be very destructive to pipe coatings. Storage life may vary from 6 months to 5 years so resistance to ultraviolet is a very important consideration. 7. Ability to maintain substantially constant electrical resistivity with time. The ef- fective electrical resistance of a coating per average square foot depends on the following. • Resistivity of the coating material • Coating thickness • Resistance to moisture absorption • Resistance to water vapor transfer • Frequency and size of holidays • Resistivity of the electrolyte • Bond or adhesion of coating If the effective resistance is unstable, the CP required may double every few years. It is easy to obtain misleading higher resistance measurements if the soil has not settled around the pipeline and if the moisture has permeated to any holidays in the coating. Experience is necessary to evaluate the validity of these resistance measurements and to use them for designing the CP system. 8. Resistance to disbonding. Because most pipelines are cathodically protected, the coating must be compatible with CP. The amount of CP required is directly propor- tional to the quality and integrity of the coating. The negative aspects of CP are that it may drive water through the coating and that the interface bond surrounding a hol- iday may have a tendency to disbond. No coating is completely resistant to damage by CP. When large amounts of current are required, stray current and interference problems may arise. This emphasizes the importance of proper coating selection, application, and installation. 9. Ease of repair. Because the perfect pipe coating does not exist, we can expect to make some ﬁeld repairs as well as ﬁeld-coating of the weld area. Check for compatibility and follow the manufacturer’s recommendations. A ﬁeld repair is never as good as the original coating. Tight inspection should be maintained.10. Nontoxic interaction with the environment. Some coating materials have been mod- iﬁed, restricted, or banned because of environmental and health standards. Asbestos felts and primers with certain solvents have required substitution of glass rein- forcements and modiﬁcation of solvents; changes in fusion-bonded epoxy powders
10 Pipeline Coatings to eliminate carcinogenic agents have also been necessitated by health and envi- ronmental concerns. This has been a major inﬂuence of change on today’s pipe coatings. In addition to the above characteristics, the following typical factors should be con- sidered when selecting a pipe coating. • Type of environment • Accessibility of pipeline • Operating temperature of pipeline • Ambient temperatures during application, storage, shipping, construction, and in- stallation • Geographical and physical location • Type of coating on existing pipeline • Handling and storage • Installation methods • Costs • Pipe surface preparation requirements Good practice in modern pipeline corrosion control work comprises the use of good coatings in combination with CP as the main lines of defense. Supplementary tactics, such as the use of insulated couplings and local environmental control may be used to reinforce these basic control methods. In selecting a coating system for a given pipeline project, one of the most important characteristics to design for is stability. By this we mean a coating combination that will have a high electrical resistance after the pipeline has been installed and the backﬁll stabilized and will lose the least electrical resistance over time. Those characteristics are important in any event but particularly so where CP is used to supplement the coating. When used with an unstable coating, a CP system that is fully adequate during the early life of a pipeline may no longer provide full protection as the coating deteriorates (as indicated by a reduction in the effective electrical resistance of the coating), which will require additional current. This means that continued expenditures will be necessary for additional CP installations. The overall economics of the coating- plus-CP concept are adversely affected by poor coating performance. In a review of 50 years of literature on pipeline coatings, the following concepts emerged: • Selection of the best coating and proper application are very important. • CP must supplement the coating for 100% protection. • In-the-ground tests are more reliable than laboratory tests. • Results of adhesion tests do not correlate with those of cathodic disbondment tests. • Cathodic disbondment tests are the best tests to measure coating performance. • The current required for CP is the best measure of coating performance.
Speciﬁcations 11 • Optimum coating thickness is important. • Soil stress is one of the main problems. • Resistance to cathodic disbondment and soil stress are very important requirements of a pipe coating. For a pipe coating to be effective, it should meet these criteria: adhesion, adequate thickness, low moisture absorption/transfer, chemical resistance (especially alkalis from CP), and ﬂexibility. • Selection of the best appropriate system is important, but proper application is the most important consideration. A major cause of pipeline coating failure is improper application. A quality material poorly applied is of little value, and the quality of a pipe coating is only as good as the quality of application. To assist in the evaluation of an applicator, the following points should be considered. 1. Experience. Research and trial and error have gone into the development of every coating, with close cooperation between applicator, coating manufacturer, equipment manufacturer, and customer. The transition from laboratory to production line is usu- ally a costly experience, which should not be ignored. 2. Reputation. This is an asset earned by consistent performance. Not only good quality work but also solving problems and correcting mistakes help to develop a reputation. 3. Reliability. Many variables affect the application of coatings. A reliable work force, well-maintained equipment, and consistent quality performance are prerequisites for an applicator. 4. Conformance to the coating manufacturer’s speciﬁcations. The manufacturer’s es- tablished minimum speciﬁcations for application of materials should be met. 5. Modern automated equipment. Capital expenditure on automated application equip- ment is an important part of the success of plastic coatings. Elimination of human er- rors through automation and controls continues to be an important factor in improved pipe coatings. 6. Quality control. Conformance to speciﬁcations has to be checked regularly. Knowl- edge of the applicator’s quality control procedures on materials, application, and ﬁnished product is essential in the selection of an applicator.SPECIFICATIONS Pipeline coating should not be attempted without rigid speciﬁcations that precisely spell out every step of the coating procedure to be used. Such speciﬁcations are necessary to ensure that the materials being used are applied in a manner that will permit develop- ment of the best coating of which those materials are capable. Because many materials may be used, no speciﬁc example of coating speciﬁca- tions will be attempted here. Speciﬁcations can be prepared in accordance with the
12 Pipeline Coatings manufacturer’s recommendations with such modiﬁcations as may be dictated by con- ditions applicable to the particular project and requirements of the pipeline system in which the coated pipe is to be used. Areas to be covered by speciﬁcations should include the following. • Cleaning the pipe surface • Priming, if required • The coating materials to be used and (if more than one material) the order in which they are to be applied • Total thickness with permissible tolerances • Speciﬁcations applicable to the particular materials to be used, such as application temperature and thickness, tension (for tapes or wrappers), and other items of a similar nature • Handling requirements for coating materials, such as storage provisions and mainte- nance of dry and clean conditions • Inspection requirements • Procedure for repair of coating defects • Basis for rejection of unacceptable coating • Requirements for handling and transporting the coated pipe • Details of coating ﬁeld joints when factory coated pipe is used • Backﬁlling requirementsINSPECTION PROCEDURES Once the coating system and applicator are selected, an important part of a quality installation is good inspection. Inspection should begin with the stockpile of bare pipe through coating operations, load out, coated pipe stockpile, ﬁeld inspection, joint coating procedure, and backﬁll of coated pipe. Knowledge of the coating system, plant facilities, quality control methods, shipping requirements, handling, joint coating, ﬁeld conditions, ﬁeld holiday detection, and repair are requirements for proper installation. Experience and common sense in interpretation of speciﬁcations and analysis of test results will contribute to obtaining the best possible coating results. As a ﬁnal backup to application supervision exercised by the coating inspector, usual pipelining practice includes a ﬁnal test with a holiday detector (or “jeep”). This device impresses an electrical voltage across the coating. An electrode is passed over the entire coating surface and, as it passes over a coating defect, there is an electrical discharge between electrode and pipe. This discharge, or spark, actuates a signaling device, which warns the operator that a holiday has been detected. The operator marks the defect for the repair crew and continues. Refer to the proper NACE speciﬁcation when examining for holidays: RP02-74 (latest revision) for the thicker coatings, or RP04-95 (latest revision) for the thinner coating systems.
Inspection Procedures 13Plant Holiday Inspection Pipe coated at a coating plant normally is passed through a holiday detector before shipment. Both mill-coated pipe and that coated over the ditch should be subjected to a ﬁnal holiday test before being placed in the ditch. The fewer the defects in a coating which is to be repaired, the better the quality of the completed coating. Nevertheless, if all holidays are picked up by a detector in proper operating conditions, and if they are repaired to conform to an effective procedure, then the quality of the coating as it enters the ditch will at least approach an optimum.Field Holiday Inspection Several types of holiday detectors are suitable for ﬁeld use at the pipeline construction site. The most common ones are usually battery operated and equipped with some type of pipe-encircling electrode. The electrode is arranged so that the ring may be pushed or rolled along the pipe by the operator, allowing the electrode to sweep all portions of the coating surface. The holiday detector should be operated in strict accordance with the manufacturer’s instructions. The coating inspector should be sure the operator has been trained properly and is using the equipment correctly. Some practical operating procedures that apply to any type of holiday locator include the following. 1. Use only adequately charged batteries in battery-operated models. 2. Use detectors that are set to operate at a voltage suitable for the coating being applied. Thick coatings require a high voltage to spark through at defects. On the other hand, too high a voltage may break down thin ﬁlm coatings such as tapes or other thin plastic coatings. 3. Verify periodically that the detector is operating properly. This may be done by purposely making a coating defect (such as a pinhole made with a knife) and pass- ing the detector over the hole. Failure to detect the hole properly indicates the need for prompt corrective adjustment. During production work, veriﬁcation should be made at least twice a day and at such other times as the inspector may suspect poor performance. 4. Keep the contact electrodes clean. A buildup of coating material on electrodes may interfere with efﬁcient detection or even prevent it entirely. This possibility is greater with some materials than others. Where found to be a factor, keeping the electrodes clean of the insulating coating material must be insisted on. 5. Maintain a good ground. To be complete, the detector circuit must contact the earth, with a trailing ground wire for example. This trailing wire should be checked for damage daily (or whenever faulty detector operation is suspected) and replaced or repaired if faulty. When working on long sections of line, there usually will be sufﬁcient
14 Pipeline Coatings conductance between line and earth to permit adequate detector operation. On the other hand, a short length of well-coated pipe on dry skids may have to be grounded to the pipe to establish an adequate circuit.TYPES OF PIPELINE COATINGS The types of pipeline coatings and their characteristics are summarized in Table 2.1.Table 2.1 Types of Pipeline CoatingsPipe coating Desirable characteristics LimitationsCoal tar enamels 80+ years of use Limited manufacturers Minimum holiday susceptibility Limited applicators Low current requirements Health and air quality concerns Good resistance to cathodic disbondment Change in allowable reinforcements Good adhesion to steelMill-applied tape 30+ years of use Handling restrictions—shipping and installation systems Minimum holiday susceptibility UV and thermal blistering— storage potential Ease of application Shielding CP from soil Good adhesion to steel Stress disbondment Low energy required for applicationCrosshead-extruded 40+ years of use Minimum adhesion to steel polyoleﬁn with Minimum holiday susceptibility Limited storage (except with carbon black) asphalt/butyl Low current requirements Tendency for tear to propagate along pipe length adhesive Ease of application Nonpolluting Low energy required for applicationDual-side-extruded 25 years of use Difﬁcult to remove coating polyoleﬁn with Minimum holiday susceptibility Limited applicators butyl adhesive Low current requirements Excellent resistance to cathodic disbondment Good adhesion to steel Ease of application Nonpolluting Low energy required for applicationFusion-bonded 35+ years of use Exacting application parameters Low current requirements High application temperature Excellent resistance to cathodic disbondment Subject to steel pipe surface imperfections Excellent adhesion to steel Lower impact and abrasion resistance Excellent resistance to hydrocarbons High moisture absorptionMulti-layer epoxy/ Lowest current requirements Limited applicators extruded polyoleﬁn Highest resistance to cathodic disbondment Exacting application parameters systems Excellent adhesion to steel Higher initial cost Excellent resistance to hydrocarbons Possible shielding of CP current High impact and abrasion resistance
Types of Pipeline Coatings 15Enamels Bituminous enamels today are formulated from coal tar with a low carbon content, plasticized by the digestion of coal and heavy aromatic coal tar distillates followed by the addition of an inert mineral ﬁller. Petroleum asphalts with select air-blown asphalts are still used internationally as a pipe coating but their use today in North America is almost nonexistent. The early coal tar enamel (CTE) coatings usually had an outerwrap of rag felt to provide a backﬁll shield. However, the rag felt did not prevent the tendency of the CTE to creep and cold-ﬂow under soil stresses at the higher operating temperature range of the pipeline. The use of asbestos felt minimized this problem but the manufacture of asbestos wraps has been discontinued; resin-bonded glass ﬁber mats are being used at present. CTE systems have been used over 80 years, and a recently introduced two-component epoxy primer when used with special hot service enamel has increased the exposure temperature of a CTE coating system to 230 ◦ F. Today an inner and outer glass ﬁber mat are incorporated into the CTE coating system simultaneously with the application of the hot CTE. The inner glass mat is pulled into the center of the coating. The outer glass mat is usually presaturated with coal tar to assist wetting and is pulled into the outer surface of the CTE. Extra-heavy-duty outer reinforcement wraps have been developed with woven glass ﬁlaments and resin-bonded glass mats to further guard against the effects of soil stresses. The use of CTE is not expected to increase in the future because of the increased acceptance of fusion-bonded epoxy (FBE), extruded polyoleﬁn, and the FBE–polyoleﬁn combination coatings; decreasing numbers of suppliers; and restrictive regulations.Extruded Asphalt Mastic Introduced over 75 years ago, this thick (1/2 to 5/8 in [1.2 to 1.6 cm]), dense mixture of select graded sand, crushed limestone, and glass ﬁber bound with an air-blown asphalt proved to be a prominent pipe coating. Its weight, cost, and limited availability, however, led to its manufacture being discontinued.Mill-Applied Tape Coating Systems Fabric-reinforced petrolatum-coated tapes were ﬁrst used over 65 years ago. Polye- thylene tapes for pipeline coatings were introduced 46 years ago, and mill-applied tape systems were introduced 20 years ago. The mill-applied tape systems consist of a primer, a corrosion-preventative inner layer of tape, and one or two outer layers for mechanical protection. Concern regarding shielding of CP on a disbonded coating has led to development of fused multi-layer tape systems and also of a backing that will not shield CP. Environmental restrictions on solvent-based primers is being resolved by
16 Pipeline Coatings Figure 2.1 Crosshead extruded polyoleﬁn over asphaltic mastic application schematic. introducing environmentally acceptable primers. In spite of these limitations, the ready availability, ease of application, and cost mean the use of mill-applied tape systems will continue.Extruded Polyoleﬁn Systems The ﬁrst extruded polyoleﬁn system was introduced in 1956 as a crosshead-extruded polyethylene over an asphalt mastic adhesive. Originally introduced for small-diameter pipe (up to 4 1/2 in [11.4 cm]), the material is now available for pipe up to 24 in (61 cm) in diameter; the most popular size is 16 in (40.6 cm). Recent improvements in the adhesive yield better adhesion, and selection of polyethylenes has increased stress crack resistance. Available with polypropylene for use at higher temperatures (up to 190◦ F [88◦ C]), these systems have been used in Europe since the mid-1960s, along with the side extrusion method for larger diameters through 60 in (152.4 cm). A copolymer adhesive is applied to eliminate cold ﬂow and minimize shrink-back of the coating. This is followed by the application of an epoxy primer. In late 1972, the side-extrusion method was introduced in the United States. This is a dual-side extrusion, where the butyl rubber adhesive is extruded onto the pipe, followed by the polyethylene extrusion. Side extrusion can coat pipes as great as 145 in (368 cm) in diameter, the only restriction being cleaning and pipe-handling capacity. The extrusion process is a dependable production method with exacting controls. The extruder heats, melts, mixes, and extrudes the materials onto the steel pipe at the desired temperature and pressure. One may select the best polyoleﬁn to meet the end-use requirements, and the process consistently produces holiday-free
Types of Pipeline Coatings 17 Figure 2.2 Side extruded polyoleﬁn over side extruded butyl adhesive application schematic. coatings. Extrusion systems are nontoxic and do not degrade air quality. Use of these systems will continue to grow because of handleability, moisture resistance, and overall consistent reproducibility.Fusion-Bonded Epoxy Fusion-bonded epoxy (FBE) coatings were ﬁrst commercially available in late 1961. For many years they were available only on 3/4 to 8 5/8 in (1.9 to 21.9 cm) pipe but now are available in North America for pipe up to 48 in (122 cm) in diameter. For many years FBE was applied at 8–10 mil (203.2–254.0 µm) to be more competitive with other coatings. At present, it is applied at 12 mil minimum up to 25 mil (304.8–635 µm). Over the past 35 years, the resins have evolved through those requiring a primer and some requiring post application heat. None of the present epoxy pipe coatings require a primer, and most plant applications do not require post application heat. Most of the FBE pipe- coating powders have remained the same for the last 18 years. Newer dual-FBE systems were introduced in the early 1990s, to improve resistance to moisture absorption and abrasion. FBE coatings require great care to apply them properly. In addition to the NACE No. 2 near-white metal ﬁnish, a phosphate wash and demineralized water rinse have proven essential to remove potential chloride contamination and improve performance properties. Among the advantages of FBE is that it does not cover up any steel defects present, thus permitting inspection of the pipe after the FBE has been applied. Resistance
18 Pipeline Coatings Figure 2.3 Fusion-bonded epoxy powder application schematic. to soil stress and cathodic disbondment has made FBE the most speciﬁed pipe coating in the United States. The trend is to thicker applications with 16 mil (406.4 µm) being the norm. FBE will continue its prominence in the near future but will gradually share this position with improved extruded polyoleﬁn coating systems and the multi-layer (FBE–extruded polyoleﬁn) coating systems.Liquid Coating Systems Epoxy coal tars and urethanes are currently the most used liquid pipe-coating systems. They are applied in custom coating or modiﬁed plant systems, usually on larger-diameter pipes or ductile iron pipes that may not be compatible with existing pipe-coating plants. Speciﬁc manufacturers’ speciﬁcations must be strictly followed with emphasis on surface cleaning, preparation, and times for cure and overcoat. These systems are constantly evolving. The largest growth has been in the use of urethane systems.Multi-Layer Epoxy/Extruded Polyoleﬁn Systems First introduced in Europe in the mid-1960s as a hard adhesive under polyethylene, fol- lowed by the addition of an epoxy primer (FBE or liquid), multi-layer epoxy/polyoleﬁn
Conclusion 19 Figure 2.4 3–Layer copolymer coating application schematic. systems are the most-used pipe-coating systems in Europe. These systems are now avail- able throughout the world.CONCLUSION In summarizing this chapter on coatings, pipeline corrosion engineers should stress two areas of knowledge: • Full information on all details of characteristics, performance, and limitations of the coatings considered for various pipeline projects. • As complete a summary as practical of the conditions existing along the route of proposed pipeline projects together with information on the manner in which the pipeline will be operated. When well informed in these matters, corrosion engineers will be able to advise management effectively in the selection of suitable protective coating systems. They also will be able to prepare application speciﬁcations and plan inspection programs that will, if effectively implemented, ensure getting the best possible coating job.
20 Pipeline CoatingsBIBLIOGRAPHY J.D. Kellner, “Shear Strength Testing of Pipeline Coatings and Soil Stress,” Corrosion ’96, paper no. 199 (Houston, TX: NACE, 1996). NACE Standard RP0169-92, Section 5, “Coatings” (Houston, TX: NACE, 1967). A.W. Peabody, Control of Pipeline Corrosion (Houston, TX: NACE, 1967). W. Roder, Personal correspondence to R.N. Sloan, Oct 3, 1997. R.N. Sloan, “50 Years of Pipe Coatings—We’ve Come a Long Way,” Corrosion ’93, paper no. 17 (Houston, TX: NACE, 1993). R.N. Sloan and A.W. Peabody, Steel Structures Painting Council, Steel Structures Painting Manual, Vol. 1 (Pittsburgh, PA), 1982.
3 Chapter Cathodic Protection— How It Works John A. Beavers Over the years, cathodic protection (CP) has continued to be treated as a somewhat mysterious term by those not fully conversant with this most useful means of corrosion control. Apparently, many feel that CP is a complicated procedure. In actuality, the basic idea of CP is very simple. Any complications arise during the application of this basic idea. Trained pipeline corrosion engineers, however, are equipped with the knowledge needed to apply the basic concept of CP to pipeline systems and to attain a very high level of effective corrosion control. In this chapter, a simple theory of CP is described. Factors involved in application as well as limitations that must be kept in mind also are outlined. A more detailed description of the theory of CP is provided in Chapter 16.BASIC THEORY OF CATHODIC PROTECTION As deﬁned in Chapter 1, CP is a technique to reduce the corrosion rate of a metal surface by making it the cathode of an electrochemical cell. This deﬁnition is explained in greater detail here. Various conditions that cause pipeline corrosion are described in Chapter 1, and in greater detail in Chapter 16. In each case, anodic areas and cathodic areas are present on the pipe surface. At the anodic areas, current ﬂows from the pipeline steel into the surrounding electrolyte (soil or water) and the pipeline corrodes. At the cathodic areas, current ﬂows from the electrolyte onto the pipe surface and the rate of corrosion is reduced. In light of the above, it becomes obvious that the rate of corrosion could be reduced if every bit of exposed metal on the surface of a pipeline could be made to collect current. 21
22 Cathodic Protection—How It Works BURIED EARTH CONNECTION (GROUND BED) CONDUCTORS INTERCONNECTING PIPELINE, CURRENT + SOURCE OF DIRECT − CURRENT ELECTRICITY SOURCE, AND GROUND BED PROTECTED PIPELINE DOTTED LINES REPRESENT CURRENT DISCHARGE SHADED AREA ON PIPELINE FROM ANODIC AREAS DENOTES ANODIC AREAS WHICH HAS BEEN EXISTING PRIOR TO APPLICATION ELIMINATED BY OF CATHODIC PROTECTION. CATHODIC PROTECTION. Figure 3.1 Basic CP installation. This is exactly what CP does. Direct current is forced onto all surfaces of the pipeline. This direct current shifts the potential of the pipeline in the active (negative) direction, resulting in a reduction in the corrosion rate of the metal. When the amount of current ﬂowing is adjusted properly, it will overpower the corrosion current discharging from the anodic areas on the pipeline, and there will be a net current ﬂow onto the pipe surface at these points. The entire surface then will be a cathode and the corrosion rate will be reduced. This concept is illustrated in Figure 3.1. A major activity of a CP engineer is to determine the actual level of CP required to reduce the corrosion rate to an acceptable level. Monitoring, in conjunction with the application of CP criteria, are used for this determination. Details of these activities are given in Chapters 4 and 5 of this book. If, as shown by Figure 3.1, current is forced to ﬂow onto the pipe at areas that were previously discharging current, the driving voltage of the CP system must be greater than the driving voltage of the corrosion cells that are being overcome. The original cathodic areas on the pipe collect current from the anodic areas. Under CP, these same cathodic areas (which were corroding at a negligible rate in the ﬁrst place) collect more current from the CP system.
Practical Application of Cathodic Protection 23 For the CP system to work, current must be discharged from an earth connection (ground bed). The sole purpose of this ground bed is to discharge current. In the process of discharging current, the anodes in the ground bed are consumed by corrosion. It is desirable to use materials for the ground bed that are consumed at a much lower rate (pounds/per ampere/per year) than are the usual pipeline metals. This will ensure a reasonably long life for the anodes. Further discussion of ground-bed design is covered in Chapter 7.PRACTICAL APPLICATION OF CATHODIC PROTECTION With the simple theory of CP in mind, a preliminary discussion of the techniques of putting CP into actual use is given below. Details of each of these techniques are covered in later chapters.Cathodic Protection with Galvanic Anodes The corrosion cell resulting from contact of dissimilar metals is discussed in Chapters 1. In such a cell, one metal is active (negative) with respect to the other and corrodes. In CP with galvanic anodes, this effect is taken advantage of by purposely establishing a dissimilar metal cell strong enough to counteract corrosion cells normally existing on pipelines. This is accomplished by connecting a very active metal to the pipeline. This metal will corrode and, in so doing, will discharge current to the pipeline as shown in Figure 3.2. In the case of CP with galvanic anodes, CP does not eliminate corrosion; rather, it displaces corrosion from the structure being protected to the galvanic anodes. Under normal circumstances, the current available from galvanic anodes is limited. For this reason, CP by galvanic anodes normally is used where the current required for protection is small. Similarly, the driving voltage existing between pipe steel and galvanic anode metals is limited. Therefore, the contact resistance between the anodes and the earth must be low for the anodes to discharge a useful amount of current. This means that, for normal installations, galvanic anodes are used in low-resistivity soils. A normal installation, as considered here, is one in which the current from a galvanic anode installation is expected to protect a substantial length of pipeline. There are also instances where galvanic anodes are placed at speciﬁc points on a pipeline (often termed hot spots) and may be expected to protect only a few feet of pipe, especially where the line is bare. This is an application of the close anode concept, as discussed later in the chapter. Details of the design of galvanic anode installations are discussed further in Chapter 9.Cathodic Protection with Impressed Current To be free of the limited driving voltage associated with galvanic anodes, current from some outside power source may be impressed on the pipeline by using a ground bed and
24 Cathodic Protection—How It Works DRIVING VOLTAGE CAN BE WORKING GALVANIC DEMONSTRATED BY CONNECTING ANODE OF ZINC OR ANODE AND UNPROTECTED MAGNESIUM BURIED IN PIPELINE TO VOLTMETER AS EARTH AND CONNECTED SHOWN. TYPICALLY, PIPELINE TO PIPELINE WITH WIRE COULD BE APPROXIMATELY WILL DISCHARGE CURRENT 1.0 VOLT POSITIVE TO AND PROTECT PIPELINE MAGNESIUM ANODE AND AS SHOWN. 0.5 VOLT POSITIVE TO ZINC ANODE. V (−) (+) PROTECTED UNPROTECTED PIPELINE. PIPELINE. Figure 3.2 Cathodic protection with galvanic anodes. a power source. Figure 3.1 illustrates this situation. The most common power source is the rectiﬁer. This device converts alternating current (AC) electric power to low-voltage direct current (DC) power. Rectiﬁers usually are provided with the means for varying the DC output voltage, in small increments, over a reasonably wide range. Although the maximum output voltage may be less than 10 V or close to 100 V, most pipeline rectiﬁers operate in the range between 10 and 50 V and can be obtained with maximum current outputs ranging from less than 10 A to several hundred amperes. This serves to illustrate the ﬂexibility in choice of power source capacity available to the corrosion engineer when planning an impressed current CP system. Any other reliable source of DC electric power can be used for impressed current CP systems. Some of these are discussed in Chapter 10. Details of the design of rectiﬁer installations are treated in Chapter 8.Criteria for Cathodic Protection Although the basic theory of CP is simple (impressing DC on a structure to reduce the corrosion rate), the obvious question that arises is: How do we know when we have attained adequate protection on a buried structure? The answer to this question is that various criteria have been developed over the years that permit a determination of whether adequate protection is being achieved. Those criteria in more common usage involve measuring the potential between the pipeline and earth. The measurement per- mits a rapid and reliable determination of the degree of protection attained. Basically,
Practical Application of Cathodic Protection 25 potential criteria are used to evaluate the changes in structure potential with respect to the environment that are caused by CP current ﬂowing to the structure from the surrounding soil or water. The potential measurement criteria, as well as other criteria, are discussed in detail in Chapter 4. The potential of a pipeline at a given location is commonly referred to as the pipe- to-soil potential. The pipe-to-soil potential can be measured by measuring the voltage between the pipeline and a reference electrode placed in the soil directly over the pipeline. The most common reference electrode used for this purpose is a copper-copper sulfate reference electrode, which is commonly given the acronym CSE. The potential is referred to as an on potential if the measurement is made with the CP system energized. The off or instant off potential estimates the polarized potential when the measurement is made within one second after simultaneously interrupting the current output from all CP current sources and any other current sources affecting that portion of the pipeline. See Chapters 4 and 5 for further details on potential measurements.Selection of Type, Size, and Spacing of a Cathodic Protection System Some of the questions to be resolved when planning a pipeline CP system include the following: 1. Shall galvanic anodes be used or would an impressed current system be a better choice? 2. How much total current will be required to attain adequate CP? 3. What should be the spacing between installations, and what will be the current output required from each installation? 4. What provisions should be made to permit testing the completed installation? 5. Are there special conditions at certain locations that will require modiﬁcations in the general plan for CP? These questions cannot be answered using only material covered up to this point. The needed information that will inﬂuence the decision includes such items as: • The corrosivity of the environment; • The soil structure and resistivity; • Whether the pipeline is bare or coated; • If coated, the quality and electrical strength of the coating and the presence of envi- ronmental conditions that may cause the coating to deteriorate; • The metal or alloy used in the pipeline; • The size of the pipeline and its ability to conduct CP current; • The presence of metallic structures from other resources (usually termed foreign struc- tures) crossing or close to the pipeline to be protected; • The presence of stray current from man-made or natural sources.
26 Cathodic Protection—How It Works As this list makes apparent, an appreciable quantity of information and data must be accumulated with respect to the pipeline for which CP is planned. Once reliable information is obtained in sufﬁcient detail, answers to the questions posed earlier in this section can be developed and a sound engineering design can be prepared. Chapters 5 through 12 are concerned with getting the needed data and using it in the CP design.Effect of the Coating on Cathodic Protection In the discussion of coatings in Chapter 2, it was stated that better than 99% of the surface of a well-coated pipe would be completely free of corrosion. Also, it was stated that CP would be relatively easy to apply because only minute areas of exposed steel would require protection. Let us look at these statements again and get an idea of their signiﬁcance in terms of the amount of current that must be supplied for CP. Figure 3.1 illustrates the pattern of current ﬂow that is expected for protection of a section of bare pipeline. The picture is quite different with a high-resistance barrier coating between the pipeline and the environment, as illustrated by Figure 3.3. In Figure 3.3, current from the CP ground bed is shown ﬂowing to all areas where pipe metal is exposed. In so doing, the original corrosive current discharge from defects in anodic areas is reduced. In addition to the current shown ﬂowing to defects, current also ﬂows through the coating material itself. No coating material is a perfect insulator (even when absolutely free of any defects whatsoever) and will conduct some current. The amount will depend on the electrical resistivity of the material (expressed in ohm-cm) and its thickness. When a high-resistivity coating is used, the current passing directly GROUND BED + − POWER SOURCE PIPE SHOWN IN CROSS SECTION COATING MATERIAL Figure 3.3 Cathodic protection of a coated pipeline.
Practical Application of Cathodic Protection 27 Table 3.1 Range of Current Required for Protection of 10 Miles of 36-in Diameter Pipe (under conditions stated in text) Effective coating resistance in ohms for one average square foot Current required in amperes Bare Pipea 500 10,000 14.91 25,000 5.964 50,000 2.982 100,000 1.491 500,000 0.2982 1,000,000 0.1491 5,000,000 0.0298 Perfect coating 0.000058 a Bare pipe assumed to require a minimum of 1 mA/ft2 .through the coating will be negligible compared with that ﬂowing to coating defectsunless the number and size of the defects are unusually small. Table 3.1 gives some idea of the CP current range that may be encountered. Thecurrent required to protect a 10-mile section of 36-in diameter pipeline is compared fora wide range of coating resistances, from bare pipe to a holiday-free coating 3/32 inthick with a resistivity of 1 × 1013 ohm-cm. The pipeline section is assumed to be in soilhaving an average resistivity of 1 × 103 ohm-cm. The current required is that needed tocause a 0.3 V drop across the effective resistance between the pipeline and remote earth(polarization effects are neglected). The effective coating resistances given in Table 3.1 all could be obtained with the samecoating for which the perfect coating current ﬁgure is given but with varying numbersof coating defects. For the examples used in the table, effective resistances of 1 × 104 to2.5 × 104 ohms for one square foot of coating reﬂect either poor handling and installationof the coated pipe or degradation of the coating after installation. For pipelines in 1 × 103ohm-cm soil, average resistances of 1 × 105 to 5 × 106 ohms for one square foot of coatingindicate good to superior construction work and little or no degradation of the coatingwith time. The table shows that a bare pipeline can accept thousands of times more currentthan the same line with a superior coating. An ordinary two-cell ﬂashlight bulb draw-ing ∼0.5 A can take nearly 17 times as much current as that required to cathodicallyprotect 10 miles of 36-in diameter pipe with a superior coating (5 × 106 ohms for onesquare foot). In contrast, the current required to protect a line with a poorly appliedcoating (2.5 × 104 ohms for one square foot) could be at least 200 times more than thecurrent required if the same coating were applied and handled in a superior manner.The examples given are meant to stress a most important point. Because of the widevariation possible, the pipeline corrosion engineer must know the present condition ofthe coating on the pipeline before determining how much current will be needed from a
28 Cathodic Protection—How It Works proposed CP system. The engineer also must be able to estimate the rate of degradation of the coating so that the CP system can be designed to protect the pipeline as the coating degrades. Very long lengths of pipeline can be protected with a single CP system. For example, it is frequently possible to protect over 50 miles of cross-country pipeline from one location, if the pipeline has a large-diameter and is well coated. Oddly enough, it is easier to protect long lengths of large-diameter pipe than of small-diameter pipe from a single CP installation. In a CP installation such as that shown in Figure 3.1, current ﬂow at any location on the pipe is inversely proportionally to the total resistance of the system at that location, based on Ohm’s law. Once the current enters the mass of the earth from a ground bed, it is in a very low resistance conductor and theoretically will travel great distances if there is a suitable return conductor. In pipeline work, the pipe itself is the return conductor. For a given wall thickness, large-diameter pipe has a lower resistance than small-diameter pipe because the former has a larger cross-sectional area and the resistance of a conductor is inversely proportional to the cross-sectional area. Therefore, a larger-diameter pipe will permit extension of effective CP for substantially greater distances. It also follows, then, that better coatings cause less rapid buildup of current in the pipe and extend the distance of effective protection from a single CP installation.Over-Protection of Coated Lines Under some conditions, excessive amounts of CP current to a coated pipeline may dam- age the coating. This process is called cathodic disbondment. The current ﬂow promotes water and ion migration through the coating and an increase in the electrolyte pH at the pipe surface. If the polarized potential is sufﬁciently negative, hydrogen can also evolve in the form of gas bubbles on the pipe surface. All of these processes are detrimental to coatings and promote degradation and disbondment. The polarized potential at which signiﬁcant damage to a coating occurs is a function of many factors, including the inherent resistance of the coating to degradation, the quality of the coating application, the soil conditions, and the pipeline temperature. As a rule of thumb, off-potentials that are more negative than −1.1 V (CSE) should be avoided to minimize coating degradation. In this connection, it should be noted that damaging conditions can be created readily by an improperly adjusted impressed current CP system, and can sometimes result when using high-potential galvanic anodes such as magnesium, but seldom if ever will develop when using low-potential galvanic anodes such as zinc.Remote vs Close Ground Beds Flow of current from an external source to a pipeline (as is true when the pipeline is cathodically protected) will be accompanied by a potential difference between the earth
Practical Application of Cathodic Protection 29 and the pipeline, the earth being positive (+) and the pipeline negative (−). The potential difference is used in certain criteria for determining the degree of CP, as will be covered in Chapter 4. Developing the desired potential difference can be accomplished in either of two ways: • By making the pipeline negative with respect to remote earth, or • By making the earth positive with respect to the pipe in local areas. The ﬁrst method uses remote ground beds, from which substantial lengths of pipeline can be protected. The second method uses close ground beds or anodes, which afford protection only in their immediate vicinity.Remote Ground Beds The sketch in Figure 3.1 may be used yet again to illustrate the remote ground bed type of installation. Current discharge, from an anode or group of anodes forming the ground bed, will cause voltage drops in the earth between points along lines radiating from the ground bed. Close to the ground bed, the voltage drop per unit of distance is relatively high. As one moves away from the ground bed, this voltage drop per unit of distance becomes less and less until a point is reached beyond which no further signiﬁcant voltage drop can be observed. This point may be considered as remote earth and establishes the radius of what is termed the area of inﬂuence surrounding the ground bed. Exactly as described above, current ﬂowing to the protected pipeline also will cause a voltage drop in the soil adjacent to the line, and there will be an area of inﬂuence surrounding the pipeline. The ground bed shown in Figure 3.1 may be said to be remote from the pipeline if it is far enough away such that there is no signiﬁcant overlap between the area of inﬂuence surrounding the ground bed and the area of inﬂuence surrounding the pipeline. Under such conditions, current ﬂows from the ground bed into the general mass of the earth, which may be considered a resistance-less, or inﬁnite, conductor. Cur- rent will then ﬂow from this inﬁnite conductor to the pipeline to be protected and cause a voltage drop across the resistance between the pipeline and this inﬁnite conductor. The simple equivalent circuit shown in Figure 3.4 illustrates this concept. Under these conditions, the pipeline will be made negative with respect to remote earth and, if made sufﬁciently negative, effective CP will result. With current ﬂowing in an inﬁnite conductor as illustrated, the resistance of the pipeline itself may limit the length of pipeline that can be protected from one ground bed. As described above, pipelines having lower incremental longitudinal resistances (large diameter lines) can have longer sections protected from one ground bed, other conditions being equal. A limitation at the most remote point from the ground bed is the minimum potential required for adequate CP. A limitation near the ground bed is the need to maintain the pipe-to-soil polarized potential at values that are less negative than about 1.1 V (CSE) to avoid coating damage and hydrogen effects in susceptible steels.
30 Cathodic Protection—How It Works RESISTANCE, GROUND GROUND BED BED TO REMOTE (+ WITH RESPECT EARTH. TO REMOTE EARTH). + INFINITE (RESISTANCE- LESS) CONDUCTOR − REPRESENTING REMOTE EARTH. PIPELINE INCREMENTIAL INCREMENTIAL PIPELINE RESISTANCE, RESISTANCE + − PIPELINE TO POWER REMOTE EARTH. SOURCE Figure 3.4 Simple equivalent circuit of a pipeline with a re- mote ground bed.Close Ground Beds The use of close anodes, or a series of anodes, is quite different from the remote type of installation just described. Their successful use depends on the area of inﬂuence sur- rounding each ground bed anode as has been discussed in general terms. For a better understanding of how close anodes are used, the conductive path between a ground bed anode and remote earth is examined in greater detail. The current per unit of cross-sectional area of earth (current density) ﬂowing away from a ground bed anode is highest close to the anode and decreases with distance. Where the current density is highest, the greatest point-to-point potential drops can be observed in the earth. The net result of this effect is that most of the potential drop to remote earth of a single anode normally is encountered within the ﬁrst few feet. This is illustrated by Figure 3.5, which shows the percentage of the total resistance or potential drop (with respect to remote earth) as a function of distance from an anode that is discharging current. The curves in Figure 3.5 are based on a 3-in diameter × 60-in long anode discharging 2 A of current in 1×103 ohm-cm resistivity soil. Other anode sizes will result in somewhat different shaped curves, but the one illustrated is typical. Non-uniform soil conditions also will change the shape of the curve. The curve is based on the following formula from Rudenberg (1945): 0.038Iρ (y + y2 + x 2 ) Vx = log10 (1) πy x where: Vx = Potential at x (see Figure 3.5) in volts caused by ground anode current I = Ground anode current in amperes